J. Phys. Chem. C XXXX, xxx, 000 A
Hydrophilic Monodisperse Magnetic Nanoparticles Protected by an Amphiphilic Alternating
Eleonora V. Shtykova,† Xinlei Huang,‡ Xinfeng Gao,‡ Jason C. Dyke,‡ Abrin L. Schmucker,‡
Bogdan Dragnea,‡ Nicholas Remmes,§ David V. Baxter,§ Barry Stein,| Peter V. Konarev,†,⊥
Dmitri I. Svergun,*,†,⊥ and Lyudmila M. Bronstein*,‡
Institute of Crystallography, Russian Academy of Sciences, Leninsky pr. 59, 117333 Moscow, Russia,
Department of Chemistry, Indiana UniVersity, 800 East Kirkwood AVenue, Bloomington, Indiana 47405,
Department of Physics, Indiana UniVersity, 727 East Third Street, Bloomington, Indiana 47405, Department of
Biology, Indiana UniVersity, 1001 East Third Street, Bloomington, Indiana 47405, EMBL, Hamburg Outstation,
Notkestra e 85, D-22603 Hamburg, Germany
ReceiVed: June 18, 2008; ReVised Manuscript ReceiVed: August 8, 2008
Iron oxide nanoparticles (NPs) with diameters of 16.1, 20.5, and 20.8 nm prepared from iron oleate precursors
were coated with poly(maleic acid-alt-1-octadecene) (PMAcOD). The coating procedure exploited hydrophobic
interactions of octadecene and oleic acid tails while hydrolysis of maleic anhydride moieties allowed the NP
hydrophilicity. The PMAcOD nanostructure in water and the PMAcOD-coated NPs were studied using
transmission electron microscopy, -potential measurements, small-angle X-ray scattering, and ﬂuorescence
measurements. The combination of several techniques suggests that independently of the iron oxide core and
oleic acid shell structures, PMAcOD encapsulates NPs, forming stable hydrophilic shells which withstand
absorption of hydrophobic molecules, such as pyrene, without shell disintegration. Moreover, the PMAcOD
molecules are predominantly attached to a single NP instead of self-assembling into the PMAcOD disklike
nanostructures or attachment to several NPs. This leads to highly monodisperse aqueous samples with only
a small fraction of NPs forming large aggregates due to cross-linking by the copolymer macromolecules.
Introduction robust and facile for NP hydrophilization.30-32 The encapsulation
of monodisperse iron oxide NPs by PEGylated phospholipids
Magnetic nanoparticles (NPs) have received considerable was described earlier.33,34 This method yielded exceptionally
attention because they hold promise of many exciting applica- stable and biocompatible NPs, but the high price of PEGylated
tions, such as magnetic storage media,1-3 ferroﬂuids,4-6 bio- phospholipids limits their potential applications for NP hydro-
sensors,7 contrast enhancement agents for magnetic resonance philization and stimulates the search for more affordable
imaging,8-11 bioprobes,12,13 catalysis,3 etc. Because magnetic amphiphilic molecules.
properties are size-dependent,3,14-16 obtaining narrow NP size
distribution is an important requirement in magnetic NP Alternating amphiphilic copolymers proved to be good
syntheses. Monodisperse iron oxide NPs can be prepared by candidates for NP functionalization.35,36 The hydrophilization
thermal decomposition of iron acetylacetonates1,17,18 or car- of hydrophobic nanoparticles using short (7300 Da) poly(maleic
boxylates18-20 in high-boiling solvents containing surfactants anhydride-alt-1-tetradecene) was described by Pellegrino et al.35
(oleic acid, oleylamine, etc.). As recently reported,21 the To stabilize the polymer coating, the authors used bis(6-
mechanism of thermal decomposition of a precursor (a “heating- aminohexyl)amine cross-linking the shell via interaction with
up” process) is similar to that of a “hot injection” method in anhydride moieties. Solubility in water was achieved by
separation of nucleation and growth events, leading to mono- hydrolysis of the remaining anhydride moieties. The largest NPs
disperse NPs. stabilized by this method did not exceed 9.2 nm, and no
structural studies were performed on these NPs. In the present
Typically, NPs prepared via thermal decomposition of a
paper, we report on a simpliﬁed procedure of stabilization of
precursor are hydrophobic, whereas for many applications,
large magnetic NPs (16-21 nm in diameter) with a much longer
including biomedical functions, the NPs should be hydrophilic.
alternating block copolymer (30 000-50 000 Da), poly(maleic
Several methods were suggested to hydrophilize hydrophobic
anhydride-alt-1-octadecene) (PMAOD). Interestingly, hydrolysis
nanoparticles: ligand exchange,22-26 attachment of polymer
of PMAOD in water leads to poly(maleic acid-alt-1-octadecene),
chains on nanoparticle surface,27,28 formation of NPs in the
PMAcOD, where maleic acid units are highly hydrophilic. We
presence of polymeric surfactants,29 or encapsulation of the NPs
believe that the longer copolymer chains used here provide a
with amphiphilic molecules thanks to formation of hydrophobic
stable NP shell without additional cross-linking and loss of
double layers.30-32 We believe that the last method is especially
carboxy functionality, whereas the longer hydrophobic tail (C16
* To whom correspondence should be addressed. E-mail: (L.M.B.)
vs C12 in the previously studied copolymer35) allows a more
firstname.lastname@example.org, (D.I.S.) email@example.com. stable hydrophobic double layer. In a recent paper by Di Corato
† Russian Academy of Sciences.
et al.,37 the same PMAOD was used, as well, for NP hydro-
‡ Department of Chemistry, Indiana University.
§ Department of Physics, Indiana University. philization; however, the authors again employ cross-linking
| Department of Biology, Indiana University. with an amine for coating stabilization, which we prove
⊥ EMBL. unnecessary. PMAOD was also recently used for coating of
10.1021/jp8053636 CCC: $40.75 XXXX American Chemical Society
Published on Web 10/01/2008
B J. Phys. Chem. C, Vol. xxx, No. xx, XXXX Shtykova et al.
magnetic NPs after alteration with poly(ethylene glycol) (PEG) mixture was ﬁrst heated to 60 °C to melt the solvent and allow
chains;36 however, it seems to be reasonable only for certain the reactants to dissolve under vigorous stirring. Then the
applications. temperature was increased to 370 °C with a heating rate of 3.3
In the present work, both PMAcOD self-assembling in water °C/min (using a digital temperature controller with an attached
and structure of NPs coated with PMAcOD were comprehen- Glas-Col heating mantel and set temperature of 380 °C) under
sively characterized for the ﬁrst time using small-angle X-ray vigorous stirring and reﬂuxing for 3 min. The resultant solution
scattering (SAXS), transmission electron microscopy (TEM), was then cooled down to 50 °C, and a 50 mL mixture of hexane
-potential measurements, and ﬂuorescence studies of the pyrene and acetone (volume ratio 1:1) was added into the reaction ﬂask
uptake. X-ray powder diffraction (XRD) and FTIR were used to precipitate the NPs. The NPs were separated by centrifugation
for the NP characterization. and washed three times by a mixture of hexane and acetone
Among methods providing structural information about (volume ratio 1:3). After washing, the resultant NPs were again
complex polymer or composite polymer/NP structures, SAXS centrifuged and dissolved in chloroform for long-term storage.
holds special advantages due to its capability to comprehensively (Alternatively, the solid reaction solution can be stored in a
characterize sophisticated polymer matrices, the NP size dis- refrigerator, and aggregation-free NPs can be collected and
tributions in them, and the structural changes occurring during washed directly when needed.) NP2 was prepared in a similar
the NP formation processes. Importantly, specimens are studied fashion using 1.5 mL of oleic acid. The 20.8 nm NPs (4.0%
in their natural media and aggregate states.38 In our preceding standard deviation NP3) were prepared according to the
work, we have studied structural characteristics of different kinds procedure described in our preceding papers using FeOl2 as a
of novel advanced nanomaterials at resolution from about 1 to precursor.34,52
100 nm.39-44 SAXS allowed us to obtain size distributions of 2.3. Encapsulation of Iron Oxide Nanoparticles with PMAc-
metal NPs, their locations in metal containing polymer OD. To encapsulate the iron oxide nanoparticles in PMAOD, a
matrices,39-42,45,46 and structural information about internal stock solution of PMAOD in CHCl3 was made with a
organization of the entire system.41-44 Novel methods for SAXS concentration 0.01 g/mL. The solution of 1 mg of iron oxide
data analysis originally developed for biological systems47-49 NPs in 1 mL of chloroform was added to 1 mL of the PMAOD
were for the ﬁrst time successfully applied to complex polymers solution and allowed to stir for 1 h. Chloroform was then
systems, including those containing metal nanoparticles.34,41,50,51 removed under vacuum, and 2 mL of 20% TBE buffer was
In the present paper, SAXS allows us to address the major added. Then the solution was sonicated for 10 min and heated
concern of using high molecular weight alternating copolymer: at 60 °C for an additional 10 min. Aggregates were removed
NP aggregation due to attachment of one copolymer molecule by centrifugation at 3000 rpm (twice for 15 min), and excess
to several NPs. SAXS reveals highly homogeneous populations polymer and TBE buffer were removed by ultracentrifugation
of individual NPs showing only a marginal fraction of cross- (1 h, 90 000 rpm, 4 °C), followed by ﬁltration centrifugation
linked aggregates and demonstrating that in the vast majority using 0.4 µm Millipore ﬁlters (10 min, 6000 rpm, 3 times). The
of cases, a copolymer molecule interacts with a single NP. ﬁnal product was then analyzed to conﬁrm uniformity and
absence of free polymer using TEM and DLS. The yield of the
Experimental puriﬁed particles was 90%.
2.4. Hydrolysis of PMAOD Polymer. PMAOD solution (0.8
1. Materials. FeCl3 · 6H2O (98%), and docosane (99%) were
mL, 0.01 g/mL in CHCl3) was evaporated in a vacuum oven.
purchased from Sigma-Aldrich and used as received. Hexanes
To the dried sample, 3 mL of 20% TBE buffer was added, and
(85%), ethanol (95%), and acetone (99.78%) were purchased
the solution was stirred for 72 h. The solution was then heated
from EMD and used as received. Chloroform (Mallinckrodt,
to 60 °C for 1 h and stirred at room temperature for an additional
100%), oleic acid (TCI, 95%), TBE buffer (1.3 M Tris, 450
24 h. The product was puriﬁed by dialysis against deionized
mM boric acid, 25 mM EDTA · Na2 in H2O, Fluka), and oleic
water for 24 h.
acid sodium salt (ScienceLab.com, 95%) were used without
2.5. Preparation of Samples for Fluorescence Spectroscopic
puriﬁcation. PMAOD (30 000-50 000 Da, Aldrich) was used
Analysis. To prepare the 6 × 10-7 M pyrene aqueous solution
as received. Water was puriﬁed with a Milli-Q (Millipore) water
(the concentration of a saturated pyrene solution in water is 7
puriﬁcation system (18 µS). Pyrene (98%, Aldrich) was
× 10-7 M), 10 µL of the pyrene ethanol solution (1 mg/mL)
recrystallized twice from ethanol and sublimed in vacuum at
was evaporated in a ﬂask under a ﬂow of nitrogen, and then
the ﬂask was charged with 82 mL of Milli-Q water. The resultant
2. Synthetic Procedures. 2.1. Synthesis of Iron Oxide
solution was stirred overnight in the dark.
Nanoparticles. The synthesis of iron oleate was carried out
using a published procedure.20 The resultant iron oleate was To prepare a solution containing 6 × 10-7 M pyrene and
either dried at 70 °C in a vacuum oven for 24 h (notation iron oxide NPs coated with PMAcOD, 10 µL of the pyrene
FeOl2, see ref.52) or ﬁrst extracted with ethanol and acetone ethanol solution with a concentration of 0.1 mg/mL was
to remove impurities, including oleic acid, and then dried at evaporated in a ﬂask, and then 1.65 mL of the 0.7 mg/mL
the above conditions (notation FeOl4; see ref 52). The NP3-PMAcOD aqueous solution was added, and the mixture
spherical iron oxide nanoparticles with mean diameters of was stirred for 24 h in the dark. In addition, the above solution
16.1 nm (3.7% standard deviation, NP1) and 20.5 nm (4.1% was diluted with a 6 × 10-7 M pyrene aqueous solution to obtain
standard deviation, NP2) were synthesized using thermal the ﬁnal solutions with concentrations of 0.35, 0.07, and 0.007
decomposition of FeOl4.53 In a typical experiment for NP1, mg/mL. Each solution was stirred for 24 h in the dark for
1.39 g (1.5 mmol for the molecule containing three oleates equilibration.
per one Fe) of FeOl4, 1.6 mL of oleic acid (5 mmol), and 3. Characterization. FTIR spectra were recorded on a
7.7 g of docosane (hydrocarbon C22H46, solid at room temper- Nicolet spectrometer by placing the sample on a KBr disk and
ature) were mixed in a three-neck, round-bottom reaction ﬂask, evaporating the chloroform or THF.
and the ﬂask was degassed four times using “evacuation-ﬁlling -Potential measurements were performed using a Malvern
with argon” cycles, ending with ﬁlling with argon. Then the Zetasizer Nano ZS equipped with an MPT-2 autotitrator
Magnetic Nanoparticles J. Phys. Chem. C, Vol. xxx, No. xx, XXXX C
and S (sinister) indicate the conﬁguration of the corresponding
chiral carbon. In the second step, each model of the -MAcOD-
unit was solely used to build a short PMAcOD polymer chain
consisting of 10 -MAcOD- units with an extended conforma-
tion, generating eight models of the PMAcOD polymer chain
correspondingly. Energy minimization was carried out for each
PMAcOD polymer model. The resulting structures of the short
PMAcOD polymer chain were consequently used to construct
models of self-association of this polymer in solution. These
structures were taken into use in two ways: (i) a structure was
entirely taken as a building block or (ii) a structure fragment of
one -MAcOD- unit was taken from the structure and used as
a basic building unit. Bilayer assemblies of different geometrical
shapes were constructed, and their SAXS patterns were calcu-
lated using the program CRYSOL48 and compared with the
Figure 1. -Potential as a function of pH for PMAcOD and NP1 and experimental scattering to ﬁnd the overall organization of the
NP3 coated with PMAcOD. alternating copolymer in solution best ﬁtting the SAXS data.
The agreement between the experimental data Iexp(s) and those
calculated from the models was characterized by the discrepancy
containing HCl (0.1 M and 0.01 M) and NaOH (0.1 M). The
Iexp(sj) - cIcalc(sj) 2
software was programmed to titrate the solutions from pH 7.5 1
down to pH 2.5-3 in increments of 0.5 pH. -Potential and N-1 j
pH values were measured before and after sample recirculation
through the folded capillary cell. Data was processed using the where N is the number of experimental points, c is a scaling
absorption of bulk iron oxide, the indices of refraction of iron factor and Icalc(sj) and σ(sj) are the calculated intensity and the
oxide and solvent, and the viscosity of the pure water. The experimental error at the momentum transfer sj, respectively.
Smoluchowski approximation was used to convert the electro- Magnetic measurements were carried out using a Quantum
phoretic mobility to a -potential. Design MPMS XL magnetometer. Zero-ﬁeld cooling curves
Electron-transparent specimens for TEM were prepared by were taken by cooling the sample in null ﬁeld ((0.1 Oe) down
placing a drop of a dilute solution onto a carbon-coated Cu grid. to 4.5 K, applying a 50 Oe ﬁeld, and then measuring the
Images were acquired at an accelerating voltage of 80 kV on a magnetization in regular temperature increments up to 300 K.
JEOL JEM1010 transmission electron microscope. Images were For the FC curves, the samples were cooled in the 50 Oe ﬁeld
analyzed with the Adobe Photoshop software package and the to 4.5 K and magnetization measurements were repeated in
Scion Image Processing Toolkit to estimate NP diameters. regular temperature increments up to 300 K.
Normally, 150-300 NPs were used for analysis. Fluorescence spectra were recorded on a Perkin-Elmer LS-
X-ray diffraction patterns were collected on a Scintag theta- 50B luminescence spectrometer equipped with a thermo NESLAB
theta powder diffractometer with a Cu KR source (0.154 nm). RTE-140 low-temperature bath circulator for temperature
The synchrotron radiation X-ray scattering experiments were control. All measurements were carried out at 25 °C unless
performed on the X33 camera54 of the European Molecular stated otherwise. For measurements of the emission spectra, the
Biology Laboratory (EMBL) on the storage ring DORIS III of excitation and emission slits were set at 5 and 3.5 nm,
the Deutsches Elektronen Synchrotron (DESY, Hamburg). A respectively. The excitation wavelength was set at 330 nm, and
MAR Image plate detector was used to collect the scattering spectra were recorded from 350 to 550 nm with a scan rate of
data in the range of the momentum transfer 0.1 < s < 5.0 nm-1, 200 nm/min.
where s ) (4π sin θ)/λ, 2θ is the scattering angle, and λ )
0.15 nm is the X-ray wavelength. PMAcOD and iron oxide Results and Discussion
nanoparticles coated with PMAcOD (NP1-PMAcOD) in solu- 1. Synthesis and Characterization Using -Potential Mea-
tion were measured with exposure times of 2 min in a vacuum surements. In this work, we used three NP samples for the
cuvette to diminish the parasitic scattering. Concentrations of PMAcOD coating: NP1 (16.1 nm), NP2 (20.5 nm), and NP3
the samples in the range 0.1-1.0 mg/mL were chosen to (20.8 nm). NP1 and NP2 were prepared from the same iron
minimize interaction of the particles. Primary data processing oleate with a notation FeOl4. FeOl4 was subjected to additional
was carried out using standard procedures.55 To determine puriﬁcation to remove oleic acid uncontrollably formed during
distance distribution functions p(r) of the samples, an indirect the iron oleate synthesis and included in the iron oleate
transform program GNOM56 was used. An ab initio method of structure.52 This precursor required the addition of the increased
structural modeling (program DAMMIN 46) was employed to amount of oleic acid (capping molecules) during the NP
reconstruct the low-resolution shape and internal structure of synthesis for the successful NP stabilization (see Experimental
the iron oxide cores of the NPs. Section and the Supporting Information, SI). NP3 was prepared
The spatial structure of the -MAcOD- units of the alternat- from the other iron oleate precursor with a notation FeOl2,
ing copolymer was modeled by Cerius2 (version 3.5, MSI/ which was thermally treated after synthesis, but no oleic oleate
Accelrys).57 The ﬁrst step was to construct a single -MAc-OD- was removed.52 The TEM images and XRD spectra of the NPs
unit. Because of chirality of the two linkage carbons of the synthesized are presented in (SI, Figures S1 and S2). The latter
-MAc- subunit and one linkage carbon of the -OD- subunit, demonstrate that the crystalline structure is similar in all the
the -MAcOD- unit can adopt up to eight possible conﬁgura- samples. The magnetic measurements indicate that NPs are
tions. Correspondingly, eight models were created for the superparamagnetic (see SI, Figure.S3).
-MAcOD- unit. They were designed as RRR, RRS, RSR, According to the FTIR data of the NP1 and NP3 samples
RSS, SRR, SRS, SSR, and SSS, respectively where R (rectus) (see SI, Figure S4 for details), the former NPs contain a larger
D J. Phys. Chem. C, Vol. xxx, No. xx, XXXX Shtykova et al.
Figure 2. TEM images of NP1-PMAcOD (a) and NP3-PMAcOD (b) cast from aqueous solutions. Inset in b shows lower magniﬁcation image.
For comparative structural studies of NPs and a copolymer,
we carried out hydrolysis of PMAOD in 20% TBE buffer to
prepare PMAcOD. Because PMAcOD is an amphiphilic alter-
nating copolymer, we expected that it would self-assemble in
water, forming some ﬁnite ordered structures (see below) where
hydrophobic moieties are located in the interior of these
structures for energy minimization, whereas carboxy groups (or
carboxylates) are exposed to water. As was suggested in ref
58, self-assembling of the other amphiphilic alternating copoly-
mer, poly(maleic acid-alt-styrene) (PMAcSt), leads to formation
of stacked nanotubes.
To estimate the charges of both PMAcOD and NPs coated
with this polymer, -potential measurements were taken for
PMAcOD, NP1-PMAcOD, and NP3-PMAcOD. As can be
seen from Figure 1, the -potentials of PMAcOD and
NP3-PMAcOD are nearly the same in a wide pH range,
whereas for NP1, the -potential values are lower. Remember
Figure 3. The experimental SAXS data from PMAcOD copolymer in that in the NP1 sample, the NPs are smaller (16.1 nm) than in
solution (1) and the distance distribution function p(r) computed by NP3 (20.8 nm). We observed a similar trend for 20.1 and 8.5
GNOM (inset). The smooth curve (2) is backtransformed from p(r) nm NPs coated with carboxy-terminated PEGylated phospho-
and extrapolated to zero scattering angle. The smooth curve (3) is a lipids (see ref 33), and we believe this is caused by a different
typical best ﬁt from a disklike bilayer constructed from atomic models
NP curvature, leading to a different charge density in the NP
of individual -MAcOD- units.
exterior (lower for the smaller NPs and higher for the larger
fraction of oleic acid than the latter NPs, yet in the former case, NPs). The similarity of the -potentials of PMAcOD and
poorly adsorbed oleic acid is present (see SI, Scheme S1). Thus, NP1-PMAcOD suggests the similar charge density on the
NP1 and NP2 have similar oleic acid shell but different sizes, nanostructure surface. At pH 7, the -potential of
whereas NP2 and NP3 have similar sizes but different shell NP3-PMAcOD is about -40 mV, which is comparable to that
structures. of PEGylated phospholipid-coated NPs used as successful
We expected that the presence of the extra amount of oleic templates for Brome Mosaic Virus capsid self-assembling.33
acid in NP1 and NP2 might impede the encapsulation by Figure 2 shows TEM images of NP1 and NP3 coated with
PMAOD due to disruptions in the formation of a hydrophobic PMAcOD. This ﬁgure demonstrates that the NPs stay intact (no
double layer. The encapsulation with PMAOD was carried out etching) and do not aggregate.
by ﬁrst dissolving PMAOD in the chloroform solution of NPs, 3. Characterization by SAXS. SAXS measurements were
followed by evaporation of the chloroform and addition of 20% employed to characterize the structural organization of PMAc-
of TBE buffer with subsequent sonication, heating, and puriﬁca- OD and the NP1-PMAcOD sample in aqueous solutions. To
tion. It is noteworthy that the excess of PMAcOD (formed upon the best of our knowledge, the self-assembling of PMAcOD in
hydrolysis of PMAOD) should be removed promptly from the water was never studied before, while SAXS studies of self-
NP sample to prevent etching of iron oxide NPs. organization of other alternating amphiphilic copolymers are
To our surprise, independently of the NP type and size, stable scarce.58
NPs coated with PMAcOD were formed. We assume that in 3.1. PMAcOD Self-assembling: SAXS and Modeling. The
the presence of PMAOD, the replacement of the extra oleic acid experimental scattering proﬁle from the PMAcOD copolymer
molecules nonadsorbed on the NP surface is favored due to in solution is shown in Figure 3. The distance distribution
cooperative interactions of the PMAcOD units and the entropy function p(r) calculated from the experimental data (Figure 3,
increase. The NPs coated with PMAcOD are stable for months inset) reveals the maximum size of the particles of about 40
and do not require any additional stabilization, such as shell nm and displays negative values in the range of interatomic
cross-linking with amines.35 distances around 3-4 nm. These negative values are typical
Magnetic Nanoparticles J. Phys. Chem. C, Vol. xxx, No. xx, XXXX E
SCHEME 1: Modeling and Search for the Best Fitsa
In the ﬁgure inside the scheme: experimental scattering curve from the PMAcOD copolymer in solution (1) and the best ﬁts to the experimental
proﬁle of the scattering patterns computed from disks (2), solid (3), and hollow (4) cylinder-shape aggregates, and bicelles (5), constructed using
atomic structures of the -MAcOD- units.
for lipid bilayer structures and appear due to the hydrophobic all scattering proﬁles from the other types of models failed to
regions in the copolymer, which have a lower electron density provide good ﬁts ( > 5).
than water. The distances of 3-4 nm correspond to the double The scattering patterns calculated from all eight disklike
layer formed by the hydrophobic tails of the PMAcOD unit (1.6 structures constructed from the different conﬁgurations of the
nm for a single tail). -MAcOD- units gave very similar ﬁts. All best disklike models
To assess the organization of the PMAcODs’ self-assemblies had a diameter of 40 nm and a thickness of the bilayer of 3.2
in solution, models were constructed from the energy-minimized nm, in agreement with the results of GNOM analysis of the
single -MAcOD- units and short PMAcOD chains as de- p(r) function.
scribed in the Experimental Section. Monolayers consisting of We also attempted to construct models from the building
the -MAcOD- units in eight different conﬁgurations reﬂecting blocks consisting of 10 -MAcOD- units obtained by molecular
possible chirality of the linkage carbons were employed to modeling (see the Experimental Section and SI). The disklike
construct micelles and cylinder-shaped aggregates. Further, models with D ) 40 nm and thickness 3.2 nm again yielded
bilayered structures were employed to produce hollow cylinders, the best ﬁts, albeit showing features at higher angles that were
bicelles, and disks (Scheme 1). All of the models were not present in the experimental SAXS data (see example in the
constrained by the experimental maximum size of the aggregate SI, Figure S6). Most importantly, the modeling by short chains
Dmax ) 40 nm. The scattering intensities from the models were further conﬁrmed the shape of the self-assembled PMAcOD to
computed using CRYSOL,48, and the discrepancy was be a disklike bilayer. Similar shapes for ensembles of am-
calculated between the experimental data and the model phiphilic molecules, mostly for phospholipids, are described in
scattering. The best ﬁts obtained in each class of shapes are the literature.59-62
shown in Scheme 1. The disklike bilayers (curve 2) clearly yield 3.2. Nanoparticles Coated with PMAcOD. The experimental
the best agreement with the experimental data ( ≈ 1.9), whereas scattering proﬁle from NP1-PMAcOD in solution shown in
F J. Phys. Chem. C, Vol. xxx, No. xx, XXXX Shtykova et al.
Figure 6. Fluorescence emission spectrum of pyrene in the 0.07 mg/
mL NP3-PMAcOD aqueous solution. Inset shows the 6 × 10-7 M
Figure 4. Scattering patterns from the aqueous solution of solution of pyrene in water.
NP1-PMAcOD: experimental data (1); the curve processed by GNOM
and extrapolated to zero angle (2); scattering from the ab initio model
of the NP1 core (3); the difference scattering from the NP1-PMAcOD
aggregates (4). Insets: bottom left, distance distribution function; top
right, ab initio bead models of the individual NP core (a) and of the
cluster (b) reconstructed from the scattering data. Note that part b is
not to scale with part a, but the shape of the NP core is superposed on
the shape of the aggregate as a scale indicator.
Figure 7. Dependence of I1/I3 on the NP3-PMAcOD concentration
in aqueous solutions.
PMAcOD tails against water, and this allows one to estimate
the thickness of the hydrophobic double layer formed by
Figure 5. Comparison of the experimental SAXS proﬁles from PEG- PMAcOD + oleic acid as (22.5 - 16.0)/2 nm or (23.0 - 16.0)/2
PL-coated NPs with a diameter of 20.1 nm34 (1) and from the nm ≈ 3.2 - 3.5 nm, in agreement with the length of both
NP1-PMAcOD NPs (2). The angular axis for the former sample was hydrophobic tails partially interdigitated. No similar structures
multiplied by 0.8 to account for the difference in the sizes of the iron to those observed for pure PMAcOD in water were detected,
suggesting that inclusion of the PMAcOD molecules in the NP
shell is more favorable than their free self-assembling in the
Figure 4 (curve 1) displays distinctive maxima characteristics presence of NPs.
for practically monodisperse systems of spherical particles. The back-transformed p(r) function yielded the scattering
This scattering is dominated by the contribution from the pattern of a single NP1-PMAcOD particle (Figure 4, curve
metal, which has a much higher contrast than the amphiphilic 2), which was subtracted from the experimental SAXS data to
copolymer. The average radius of the iron oxide cores can thus yield an estimate of the scattering from the aggregates (Figure
be directly estimated from the position of the ﬁrst minimum, s1 4, curve 4). The shapes of the nanoparticles and of the
(Figure 4) as38 R ) 4.49/s1. This value was found to be 7.9 aggregates were reconstructed ab initio from the corresponding
nm, which correlates well with nanoparticle diameter of 16.0 scattering patterns by the program DAMMIN.46 A typical shape
nm from TEM. The initial portion of the SAXS pattern of the NP1-PMAcOD particle represented by an ensemble of
(scattering vectors less than s0 ≈ 0.2 nm-1) displays an upward densely packed beads (upper inset in Figure 4) yields a good
trend, indicating that a small portion of large aggregates is ﬁt to the experimental data in the range s > s0 with discrepancy
present in the NP1-PMAcOD solution. To extract the contribu- ) 1.2 (curve 3 in Figure 4). Note that the shape reﬂects solely
tion due to individual particles, the scattering pattern in the range the structure of the iron oxide core, thanks to its high positive
s > s0 was processed by the indirect transformation program contrast. The multilayered interior of the model reﬂects the
GNOM56 to compute the distance distribution function p(r) process of the formation of the iron oxide core from smaller
(Figure 4, bottom left inset). In the range of interatomic distances nuclei, as discussed in our preceding paper.34 The shape of the
below 15 nm, the bell-shaped p(r) function resembles that of a aggregates, also presented in the upper inset of Figure 4, reveals
spherical particle but at larger distances slight negative excursion an irregular conglomerate containing about 30-40 individual
is observed up to Dmax ≈ 22.5 - 23.0 nm. These negative values NP1-PMAcOD particles (in panel b, the aggregate is super-
of p(r) are clearly due to the negative contrast of the hydrophobic imposed onto the single particle). Because the zero-angle
Magnetic Nanoparticles J. Phys. Chem. C, Vol. xxx, No. xx, XXXX G
Figure 8. TEM images of NP3-PMAcOD before (a) and after (b) pyrene uptake. The TEM grids were stained with uranyl acetate to accentuate
scattering I(0) is proportional to the squared volume and the Figure 6 shows ﬂuorescence emission spectra of NP3-
volume fraction and the aggregates (curve 4) yield practically PMAcOD and of pure pyrene (inset). The I1/I3 changes from
the same I(0) value as the NP1-PMAcOD particles (curve 2), 1.71 for water to 1.39 for the 0.07 mg/mL NP3-PMAcOD
the volume fraction of the aggregates in the sample does not solution, revealing that pyrene partitions into the hydrophobic
exceed 0.1%. layer.
It is interesting to compare the present results with those Figure 7 displays a dependence of I1/I3 on the NP3-
obtained earlier for iron oxide nanoparticles encapsulated by PMAcOD concentration in aqueous solutions. Even at a concen-
phospholipids with poly(ethylene glycol) tails (PEG-PL).34 In tration of 0.007 mg/mL, some pyrene molecules have a
the latter paper, SAXS revealed dynamic clusters consisting, hydrophobic microenvironment, whereas at further dilution, the
on average, of four individual particles, and a question may NP3-PMAcOD inﬂuence on ﬂuorescence is hardly noticeable.
arise whether and how a system containing clusters of a few It is noteworthy that at NP3-PMAcOD concentrations of 0.35
particles can be distinguished from a largely monodisperse and 0.7 mg/mL, the pyrene ﬂuorescence is completely quenched.
system of individual particles containing a small fraction of large This quenching might be ascribed to close packing of pyrene
clusters. In Figure 5, the scattering from the PEG-PL-coated molecules in the hydrophobic double layer of the NP shells,
nanoparticles taken from ref 34 (curve 1) is superposed with but normally, the quenching with a neighboring pyrene molecule
the experimental scattering from NP1-PMAcOD solution results in excimer formation,66 the emission of which is not
(curve 2); the angular scale of the former pattern was multiplied observed in our case. In a control experiment, we demonstrated
by a factor of 0.8 taking into account the difference in size that the presence of PMAcOD in solution in concentrations equal
between the two types of nanoparticles). The system of the PEG- to or higher than the NP concentration of 0.7 mg/mL does not
PL-coated nanoparticles displays a characteristic scattering quench the pyrene emission, but in the solid mixed ﬁlm
proﬁle with a shoulder at small angles reﬂecting interference consisting of PMAcOD and pyrene, pyrene is partially quenched.
among the particles within the clusters, whereas the scattering We believe that the pyrene quenching in the PMAcOD shell of
from NP1-PMAcOD does not display any interference effects, iron oxide NPs should be due to a change of the pyrene packing
but shows a moderate upturn at very small angles (i.e., very conformation (compared to pure pyrene), probably combined
large sizes). One can therefore conclude that NP1-PMAcOD with adsorption and subsequent charge-transfer interaction with
NPs in solution are not cross-linked by the alternating polymer the nanocrystal, as was discussed by Turro et al. for function-
but, instead, remain largely as individual nanoparticles. alized pyrenes and γ-Fe2O3 NPs.67
4. Pyrene Uptake: Fluorescence Measurements. Because Figure 8 shows the TEM images of NP3-PMAcOD before
hydrophilization of hydrophobic NPs is carried out due to and after pyrene uptake. The TEM grids were stained with
hydrophobic interactions, it is important to evaluate the stability uranyl acetate to accentuate the shells. Because the shell exterior
of such amphiphilic shells. One might suggest that the presence is decorated with carboxyl groups, uranyl cations form clear
of hydrophobic or amphiphilic molecules in the NP solutions dark lines around NPs. The shell size calculated based on 200
might destroy the hydrophobic double layer, leading to NP NPs (in four shell locations of each particle) is 3.3 nm with a
precipitation. To investigate the stability of the hydrophobic standard deviation of 25%. This value is consistent with a double
double layer, we studied uptake of a hydrophobic molecule, layer of hydrophobic tails (fully extended oleic acid and
pyrene, using ﬂuorescence measurements.63,64 It is known that octadecene tails) with partial interdigitation, matching SAXS
pyrene has a very distinctive ﬂuorescence spectrum whose data. A close look at Figure 8a suggests that the stain penetrates
characteristics change depending on the polarity of the sur- beyond the NP exterior toward the iron oxide core, revealing
rounding medium. Typically, the ratio of the intensities of peak that the shell is not dense. After incorporation of pyrene, the
3 (I3 at 385 nm) to peak 1 (I1, 0-0 band at 374 nm)63 or vise shell size slightly increases to 3.7 nm (with a standard deviation
versa64 are used to characterize the pyrene environment. In of 6.3%), thus matching the size expected for a hydrophobic
water, I1/I3 is in the range 1.7-1.8, but in hydrophobic solvents double layer. The shell also becomes very dense, appearing
or in surfactant micelles, this value is 1.10.65 white on the TEM image (Figure 8b). This is consistent with
H J. Phys. Chem. C, Vol. xxx, No. xx, XXXX Shtykova et al.
densely packed pyrene between hydrophobic tails, leading to (15) Park, T.-J.; Papaefthymiou, G. C.; Viescas, A. J.; Moodenbaugh,
the increase in the shell density. A. R.; Wong, S. S. Nano Lett. 2007, 7 (3), 766.
(16) Rong, C.-B.; Li, D.; Nandwana, V.; Poudyal, N.; Ding, Y.; Wang,
Z. L.; Zeng, H.; Liu, J. P. AdV. Mater. 2006, 18 (22), 2984.
(17) Li, Z.; Chen, H.; Bao, H.; Gao, M. Chem. Mater. 2004, 16 (8),
Stable hydrophilic NPs were prepared by encapsulation of (18) Redl, F. X.; Black, C. T.; Papaefthymiou, G. C.; Sandstrom, R. L.;
Yin, M.; Zeng, H.; Murray, C. B.; O’Brien, S. P. J. Am. Chem. Soc. 2004,
hydrophobically coated monodisperse iron oxide NPs of 16-21 126 (44), 14583.
nm in diameter and with different surface properties using (19) Yu, W. W.; Falkner, J. C.; Yavuz, C. T.; Colvin, V. L. Chem.
alternating copolymer PMAOD. After hydrolysis, this copolymer Comm. 2004, (20), 2306.
(20) Park, J.; An, K.; Hwang, Y.; Park, J.-G.; Noh, H.-J.; Kim, J.-Y.;
forms disklike structures in water which, however, do not exist Park, J.-H.; Hwang, N.-M.; Hyeon, T. Nat. Mater. 2004, 3 (12), 891.
in the presence of NPs. In the latter case, each PMAcOD (21) Kwon, S. G.; Piao, Y.; Park, J.; Angappane, S.; Jo, Y.; Hwang,
molecule attaches mainly to the surface of a single NP, and N.-M.; Park, J.-G.; Hyeon, T. J. Am. Chem. Soc. 2007, 129 (41), 12571.
SAXS unambiguously demonstrates that 99.9% volume fraction (22) Jun, Y.-W.; Huh, Y.-M.; Choi, J.-S.; Lee, J.-H.; Song, H.-T.; Kim,
S.; Yoon, S.; Kim, K.-S.; Shin, J.-S.; Suh, J.-S.; Cheon, J. J. Am. Chem.
of NPs coated by PMAcOD are individual nanoparticles. The Soc. 2005, 127 (16), 5732.
presence of extra oleic acid on the surface of NPs does not (23) Gussin, H. A.; Tomlinson, I. D.; Little, D. M.; Warnement, M. R.;
prevent encapsulation with PMAcOD due to PMAcOD coop- Qian, H.; Rosenthal, S. J.; Pepperberg, D. R. J. Am. Chem. Soc. 2006, 128
erative interactions and an entropy increase. Fluorescence (49), 15701.
(24) Zhang, Q.; Gupta, S.; Emrick, T.; Russell, T. P. J. Am. Chem. Soc.
measurements of the pyrene uptake by NPs coated with 2006, 128 (12), 3898.
PMAcOD demonstrate that pyrene can be absorbed by the (25) Han, G.; Ghosh, P.; Rotello, V. M. Nanomedicine 2007, 2 (1), 113.
hydrophobic double layer without disintegration of the double (26) Hostetler, M. J.; Templeton, A. C.; Murray, R. W. Langmuir 1999,
15 (11), 3782.
layer, revealing a high degree of stability of the PMAcOD (27) Wan, S.; Huang, J.; Guo, M.; Zhang, H.; Cao, Y.; Yan, H.; Liu, K.
coating. J. Biomed. Mater. Res. 2007, 80A (4), 946.
(28) Kang, Y.; Taton, T. A. Macromolecules 2005, 38 (14), 6115.
Acknowledgment. This work has been supported, in part, (29) Korth, B. D.; Keng, P.; Shim, I.; Bowles, S. E.; Tang, C.;
Kowalewski, T.; Nebesny, K. W.; Pyun, J. J. Am. Chem. Soc. 2006, 128
by the NATO Science for Peace Program (Grant SfP-981438), (20), 6562.
NSF award 0631982, NIH award GM081029-01, NSF award (30) Nitin, N.; LaConte, L. E. W.; Zurkiya, O.; Hu, X.; Bao, G. J. Biol.
0220560, the IU FRSP grant, and the European Union FP6 Inorg. Chem. 2004, 9 (6), 706.
Infrastructures Program (Design Study SAXIER, RIDS 011934). (31) Dubertret, B.; Skourides, P.; Norris, D. J.; Noireaux, V.; Brivanlou,
A. H.; Libchaber, A. Science 2002, 298 (5599), 1759.
B.D. acknowledges support in part from the Indiana METACyt (32) Lim, Y. T.; Lee, K. Y.; Lee, K.; Chung, B. H. Biochem. Biophys.
Initiative of Indiana University, funded in part through a major Res. Commun. 2006, 344 (3), 926.
grant from the Lilly Endowment, Inc. The measurements at the (33) Huang, X.; Bronstein, L. M.; Retrum, J. R.; Dufort, C.; Tsvetkova,
I.; Aniagyei, S.; Stein, B.; Stucky, G.; McKenna, B.; Remmes, N.; Baxter,
EMBL beamline X33 at DESY were made within the projects B.; Kao, C. C.; Dragnea, B. Nano Lett. 2007, 7 (8), 2407.
SAXS-06-29 and SAXS-07-29. The authors thank Prof. Fran- (34) Shtykova, E. V.; Huang, X.; Remmes, N.; Baxter, D.; Stein, B. D.;
coise Winnik (University of Montreal) for helpful discussions Dragnea, B.; Svergun, D. I.; Bronstein, L. M. J. Phys. Chem. C 2007, 111
of pyrene experiments. (49), 18078.
(35) Pellegrino, T.; Manna, L.; Kudera, S.; Liedl, T.; Koktysh, D.;
Rogach, A. L.; Keller, S.; Raedler, J.; Natile, G.; Parak, W. J. Nano Lett.
Supporting Information Available: TEM, XRD, magnetic 2004, 4 (4), 703.
measurement data, FTIR, and SAXS. This material is available (36) Yu, W. W.; Chang, E.; Sayes, C. M.; Drezek, R.; Colvin, V. L.
free of charge via the Internet at http://pubs.acs.org. Nanotechnology 2006, 17 (17), 4483.
(37) Di Corato, R.; Quarta, A.; Piacenza, P.; Ragusa, A.; Figuerola, A.;
Buonsanti, R.; Cingolani, R.; Manna, L.; Pellegrino, T. J. Mater. Chem.
2008, 18 (17), 1991.
References and Notes (38) Feigin, L. A.; Svergun, D. I. Structure Analysis by Small-Angle
(1) Sun, S.; Zeng, H. J. Am. Chem. Soc. 2002, 124 (28), 8204. X-ray and Neutron Scattering; Plenum Press: New York, 1987.
(2) Frolov, G. I. Tech. Phys. 2001, 46 (12), 1537. (39) Svergun, D. I.; Shtykova, E. V.; Kozin, M. B.; Volkov, V. V.;
(3) Lu, A.-H.; Salabas, E. L.; Schueth, F. Angew. Chim. Int. Ed. 2007, Dembo, A. T.; Shtykova, E. V. J.; Bronstein, L. M.; Platonova, O. A.;
46 (8), 1222, and references therein. Yakunin, A. N.; Valetsky, P. M.; Khokhlov, A. R. J. Phys. Chem. B. 2000,
(4) Sestier, C.; Da-Silva, M. F.; Sabolovic, D.; Roger, J.; Pons, J. N. 104, 5242.
Electrophoresis 1998, 19 (7), 1220. (40) Svergun, D. I.; Kozin, M. B.; Konarev, P. V.; Shtykova, E. V.;
(5) Racuciu, M.; Creanga, D. E.; Calugaru, G. J. Optoelectron. AdV. Volkov, V. V.; Chernyshov, D. M.; Valetsky, P. M.; Bronstein, L. M. Chem.
Mater. 2005, 7 (6), 2859. Mater. 2000, 12, 3552.
(6) Bonini, M.; Wiedenmann, A.; Baglioni, P. J. Appl. Crystallogr. (41) Bronstein, L. M.; Sidorov, S. N.; Zhirov, V.; Zhirov, D.; Kabachii,
2007, 40 (S1), s254. Y. A.; Kochev, S. Y.; Valetsky, P. M.; Stein, B.; Kiseleva, O. I.; Polyakov,
(7) Chang, S. Y.; Zheng, N.-Y.; Chen, C.-S.; Chen, C.-D.; Chen, Y.- S. N.; Shtykova, E. V.; Nikulina, E. V.; Svergun, D. I.; Khokhlov, A. R. J.
Y.; Wang, C. R. C. J. Am. Soc. Mass Spectrom. 2007, 18 (5), 910. Phys. Chem. B 2005, 109, 18786.
(8) Bulte, J. W.; Kraitchman, D. L. NMR Biomed. 2004, 17, 484. (42) Shtykova, E. V.; Svergun, D. I.; Chernyshov, D. M.; Khotina, I. A.;
(9) Mulder, W. J. M.; Strijkers, G. J.; van Tilborg, G. A. F.; Grifﬁoen, Valetsky, P. M.; Spontak, R. J.; Bronstein, L. M. J. Phys. Chem. B 2004,
A. W.; Nicolay, K. NMR Biomed. 2006, 19 (1), 142. 108, 6175.
(10) Medarova, Z.; Pham, W.; Farrar, C.; Petkova, V.; Moore, A. Nat. (43) Bronstein, L. M.; Linton, C.; Karlinsey, R.; Ashcraft, E.; Stein,
Med. 2006, 13 (3), 372. B.; Svergun, D. I.; Kozin, M.; Khotina, I. A.; Spontak, R. J.; Werner-
(11) Kumagai, M.; Imai, Y.; Nakamura, T.; Yamasaki, Y.; Sekino, M.; Zwanziger, U.; Zwanziger, J. W. Langmuir 2003, 19, 7071.
Ueno, S.; Hanaoka, K.; Kikuchi, K.; Nagano, T.; Kaneko, E.; Shimokado, (44) Bronstein, L. M.; Dixit, S.; Tomaszewski, J.; Stein, B.; Svergun,
K.; Kataoka, K. Colloids Surf. B 2007, 56 (1-2), 174. D. I.; Konarev, P. V.; Shtykova, E.; Werner-Zwanziger, U.; Dragnea, B.
(12) Chemla, Y. R.; Grossman, H. L.; Poon, Y.; McDermott, R.; Stevens, Chem. Mater. 2006, 18 (9), 2418.
R.; Alper, M. D.; Clarke, J. Proc. Nat. Acad. Sci. 2000, 97 (26), 14268. (45) Svergun, D. I.; Shtykova, E. V.; Dembo, A. T.; Bronstein, L. M.;
(13) Ivkov, R.; DeNardo, S. J.; Miers, L. A.; Natarajan, A.; Foreman, Platonova, O. A.; Yakunin, A. N.; Valetsky, P. M.; Khokhlov, A. R.
A. R.; Gruettner, C.; Adamson, G. N.; DeNardo, G. L. In DeVelopment of J. Chem. Phys. 1998, 109, 11109.
tumor targeting magnetic nanoparticles for cancer therapy, NSTI Nanotech (46) Bronstein, L. M.; Platonova, O. A.; Yakunin, A. N.; Yanovskaya,
2006, Boston, MA, 2006; Nano Science and Technology Institute: Boston, I. M.; Valetsky, P. M.; Dembo, A. T.; Makhaeva, E. E.; Mironov, A. V.;
MA, 2006; pp 21. Khokhlov, A. R. Langmuir 1998, 14, 252.
(14) Talapin, D. V.; Shevchenko, E. V.; Weller, H. Synthesis and (47) Svergun, D. I. Biophys. J. 1999, 76, 2879.
Characterization of Magnetic Nanoparticles. In Nanoparticles; Schmid, G., (48) Svergun, D. I.; Barberato, C.; Koch, M. H. J. J. Appl. Crystallogr.
Ed.; Wiley-VCH: Weinheim, 2004; p 199. 1995, 28, 768.
Magnetic Nanoparticles J. Phys. Chem. C, Vol. xxx, No. xx, XXXX I
(49) Petoukhov, M. V.; Svergun, D. I. Biophys. J. 2005, 89, 1237. (59) Whiles, J. A.; Deems, R.; Vold, R. R.; Dennis, E. A. Bioorg. Chem.
(50) Shtykova, E. V.; Shtykova, E. V., Jr.; Volkov, V. V.; Konarev, 2002, 30 (6), 431.
P. V.; Dembo, A. T.; Makhaeva, E. E.; Ronova, I. A.; Khokhlov, A. R.; (60) Dubois, M.; Lizunov, V.; Meister, A.; Gulik-Krzywicki, T.;
Reynaers, H.; Svergun, D. I. J. Appl. Crystallogr. 2003, 36, 669. Verbavatz, J. M.; Perez, E.; Zimmerberg, J.; Zemb, T. Proc. Nat. Acad.
(51) Volkov, V. V.; Lapuk, V. A.; Kayushina, R. L.; Shtykova, E. V.; Sci. 2004, 101 (42), 15082.
Varlamova, E. Y.; Malfois, M.; Svergun, D. I. J. Appl. Crystallogr. 2003, (61) Gutberlet, T.; Hoell, A.; Kammel, M.; Frank, J.; Katsaras, J. Appl.
36, 503. Phys. A: Mater. Sci. Process. 2002, 74 (2), S1260.
(52) Bronstein, L. M.; Huang, X.; Retrum, J.; Schmucker, A.; Pink, M.; (62) Luchette, P. A.; Vetman, T. N.; Prosser, R. S.; Hancock, R. E. W.;
Stein, B. D.; Dragnea, B. Chem. Mater. 2007, 19 (15), 3624. Nieh, M.-P.; Glinka, C. J.; Krueger, S.; Katsaras, J. Biochim. Biophys. Acta
(53) Bronstein, L. M.; Huang, X.; Retrum, J. R.; Schmucker, A. L.; 2001, 1513 (2), 83.
Pink, M.; Stein, B. D.; Dragnea, B. Chem. Mater. 2007, 19, 3624. (63) Kalyanasundaram, K.; Thomas, J. K. J. Am. Chem. Soc. 1977, 99,
(54) Roessle, M. W.; Klaering, R.; Ristau, U.; Robrahn, B.; Jahn, D.; 72039–72044.
Gehrmann, T.; Konarev, P.; Round, A.; Fiedler, S.; Hermes, C.; Svergun, (64) Winnik, F. M.; Davidson, A. R.; Hamer, G. K.; Kitano, H.
D. J. Appl. Crystallogr. 2007, 40, s190. Macromolecules 1992, 25 (7), 1876.
(55) Konarev, P. V.; Volkov, V. V.; Sokolova, A. V.; Koch, M. H. J.; (65) Winnik, F. M.; Regismond, S. T. A. Colloids Surf., A 1996, 118
Svergun, D. I. J. Appl. Crystallogr. 2003, 36, 1277. (1/2), 1.
(56) Svergun, D. I. J. Appl. Crystallogr. 1992, 25, 495. (66) Baker, L. A.; Crooks, R. M. Macromolecules 2000, 33 (24), 9034.
(57) MSI Cerius2, Version 3.5.; Molecular Simulation Inc.: San Diego, (67) Turro, N. J.; Lakshminarasimhan, P. H.; Jockusch, S.; O’Brien,
CA, 1997. S. P.; Grancharov, S. G.; Redl, F. X. Nano Lett. 2002, 2 (4), 325.
(58) Malardier-Jugroot, C.; Van de Ven, T. G. M.; Cosgrove, T.;
Richardson, R. M.; Whitehead, M. A. Langmuir 2005, 21 (22), 10179. JP8053636